Materials 2014, 7, 5843-5857; doi:10.3390/ma7085843 OPEN ACCESS
materials ISSN 1996-1944 www.mdpi.com/journal/materials Article
Quality Assessment of Mixed and Ceramic Recycled Aggregates from Construction and Demolition Wastes in the Concrete Manufacture According to the Spanish Standard † Desirée Rodríguez-Robles *, Julia García-González, Andrés Juan-Valdés, Julia Mª Morán-del Pozo and Manuel I Guerra-Romero Superior and Technical School of Agricultural Engineering, University of Leon, Avda. Portugal 41, 24071 Leon, Spain; E-Mails: [email protected]
(J.G.-.G.); [email protected]
(A.J.-V.); [email protected]
(J.M.M.P.); [email protected]
This article is an extended version of a Conference Paper titled “Recycling of ceramic fraction of construction and demolition waste as coarse aggregate for recycled concrete production” presented at the International Conference of Agricultural Engineering CIGR-AgEng2012.
* Author to whom correspondence should be addressed; E-Mail: [email protected]
; Tel.: +34-987-291-000 (ext. 5138); Fax: +34-987-291-000. Received: 18 June 2014; in revised form: 19 July 2014 / Accepted: 7 August 2014 / Published: 13 August 2014
Abstract: Construction and demolition waste (CDW) constitutes an increasingly significant problem in society due to the volume generated, rendering sustainable management and disposal problematic. The aim of this study is to identify a possible reuse option in the concrete manufacturing for recycled aggregates with a significant ceramic content: mixed recycled aggregates (MixRA) and ceramic recycled aggregates (CerRA). In order to do so, several tests are conducted in accordance with the Spanish Code on Structural Concrete (EHE-08) to determine the composition in weight and physic-mechanical characteristics (particle size distributions, fine content, sand equivalent, density, water absorption, flakiness index, and resistance to fragmentation) of the samples for the partial inclusion of the recycled aggregates in concrete mixes. The results of these tests clearly support the hypothesis that this type of material may be suitable for such partial replacements if simple pretreatment is carried out. Furthermore, this measure of reuse is in line with European, national, and regional policies on sustainable development, and presents a solution to the environmental problem caused by the generation of CDW.
Materials 2014, 7
Keywords: characterization; composition; construction and demolition waste (CDW); ceramic aggregate; mixed aggregate; recycled concrete
1. Introduction Although the construction sector’s important contribution to the development of society is widely acknowledged, the construction industry is also perceived as a major cause of environmental degradation. Special concern rests in the European construction industry, as, besides being one of the largest consumers of natural resources—more than 50% of European natural resources , it is also a major contributor in the waste scenario—about 33% of the waste generated annually , as large quantities of the raw minerals employed end up in landfills. Consequently, the construction sector cannot remain aloof to the widespread social demand for greater respect for the environment, and must assume the task of reducing the impact caused by building work. Construction and demolition waste (CDW) constitutes an increasingly significant problem in society, not so much because of its hazardous nature, as it can be inert, but because of the volume generated, which renders sustainable management and disposal problematic. However, this waste has a very high potential for recovery, although Spain (30%) is still situated behind other European countries in terms of sustainable CDW management . Research on the use of recycled materials has become a widespread tendency. Numerous studies have investigated the possibilities of using recycled aggregates in concrete mixes as partial replacement of the conventional coarse aggregate (gravel), although the majority of them have basically focused on the use of aggregates recovered from concrete (RCA) [4–10], as their properties do not differ as much of the natural aggregates, and their use is supported by most of the standards which allow the use of secondary materials in the concrete manufacture, i.e., in Spain, the current legislation—the Spanish Code on Structural Concrete (EHE-08)  only allows this type of recycle aggregate for its inclusion up to 20% in concrete mixes, excluding the mixed recycled aggregates (MixRA), even for non-structural concretes. However, recycled aggregates obtained from crushed concrete, which despite having received most attention, only account for 15% of the CDW generated, and 30% of the CDW marketed . CDW includes a wide range of inert materials, as their composition is affected by numerous factors, including the raw materials and construction products used, the architectural techniques, and the local construction and demolition practices. Given the typical composition of CDW, there are basically two types of recycled aggregates: which are obtained from crushed concrete (RCA) and those comprising mixed components with varying percentages of ceramic material (MixRA and ceramic recycled aggregates (CerRA)). In Spain, as in other Mediterranean countries, such as Portugal, Italy, or Greece, the construction of buildings is usually based on ceramic elements combined with mortar and concrete . As determined in the Spanish National Plan of Construction and Demolition Waste 2001–2006 , one of the most significant fractions of the CDW produced is that it is composed of stone materials (bricks, roof tiles, ceramic materials and products, slabs, concrete, etc.), of which, more than half (54%) corresponds to the ceramic fraction, indicating the importance of
Materials 2014, 7
treatment and recovery of this kind of waste. Furthermore, recycled aggregates also include small amounts of other materials (impurities) depending on the origin of the waste and the treatment process carried out in the recycling plant. In this research work, as an attempt to identify a possible means of reusing this CDW, several samples of recycled aggregates with different ceramic contents were tested to assess their suitability for inclusion in concrete mixes as a partial replacement of the conventional coarse aggregate. In order to do so, the traditional method of characterizing recycled CDW aggregate was employed. This characterization was based on determining the macroscopic composition in terms of weight of the different components in the samples and measuring the key physical properties of the recycled aggregates (particle size distributions, fine content, sand equivalent, density, water absorption, flakiness index, and resistance to fragmentation). 2. Materials In this study, thirteen samples of recycled aggregates from CDW were analyzed. The samples were collected from ten CDW treatment plants located in different Spanish provinces (Figure 1). Figure 1. Spatial distribution of the recycled aggregates samples. Adapted from Google Maps .
3. Methods The characteristics of the aggregates used in the manufacture of concrete largely determine the properties of the final product. Thus, in order to get quality recycled concrete, it is necessary that the recycled aggregates used meet the requirements of the standard UNE-EN 12620:2003 + A1: 2009  and the Chapter VI: Materials of the EHE-08 .
Materials 2014, 7
In order to perform the characterization of the recycled aggregates, a representative quantity of all the samples was selected, following the specifications in UNE-EN 932-1:1997 , and was subjected to the following tests: composition content (UNE-EN 933-11:2009/AC:2010 ), particle size (EHE-08  and UNE-EN 933-1:2012 ), quantity of fines (EHE-08 ), sand equivalent (UNE-EN 933-8:2012 ), flakiness index (UNE-EN 933-3:2012 ), density and water absorption (UNE-EN 1097-6:2001/A1:2006 ) and Los Angeles test (UNE-EN 1097-2:2010 ). Finally, by comparing the results obtained and the guidelines established by the aforementioned Spanish standards, it was possible to assess the suitability of the materials for use as recycled aggregate in concrete manufacturing. 4. Results and Discussion 4.1. Composition The constituents found in the recycled coarse aggregates (4/40 mm) are shown in Table 1. Table 1. Composition of recycled aggregates (coarse fraction) from construction and demolition waste (CDW), based on UNE-EN 933-11 . Rc: concrete, mortar and natural aggregates with mortar attached; Ru: unbound natural aggregates without mortar attached; Rb: ceramics (brick, tiles…); Rg: glass; Ra: asphalt; X1: gypsum; and X2: other impurities (wood, plastic, metals). Sample a CDW1 CDW2 CDW3 CDW4 CDW5 CDW6 CDW7 CDW8 CDW10 CDW11 CDW12 CDW13 Mean Standard deviation Maximum Minimum
Rc 49.14 28.67 33.07 46.69 56.41 14.03 44.11 32.01 36.35 12.76 46.86 34.62 36.23 13.45 56.41 12.76 a
Ru 29.47 33.91 37.65 20.02 18.08 45.44 17.51 42.69 9.33 21.38 23.83 38.72 28.17 11.47 45.44 9.33
Rb 16.51 33.56 28.43 31.41 23.96 38.08 33.56 21.42 49.89 64.75 24.08 21.91 32.30 13.58 64.75 16.51
Rg 0.17 0.11 0.04 0.08 0.00 0.00 0.75 0.58 0.01 0.00 0.00 0.00 0.14 0.25 0.75 0.00
Ra 4.38 0.83 0.29 1.33 1.18 1.35 0.44 1.02 0.17 0.86 1.05 3.10 1.33 1.22 4.38 0.17
X1 0.09 2.64 0.22 0.34 0.21 0.65 3.48 1.84 4.12 0.12 3.81 1.55 1.59 1.56 4.12 0.09
X2 0.25 0.28 0.31 0.14 0.16 0.45 0.16 0.44 0.13 0.14 0.35 0.10 0.24 0.12 0.45 0.10
Results of Sample CDW9 are not available.
The recycled aggregates were composed of the following materials: concrete and mortar, natural aggregates, ceramics, asphalt, glass, gypsum, and impurities, such as wood, plastic, and metal. The data showed that the predominant material was concrete, with mean values of 36.23%, followed by materials of a ceramic nature, which constituted 32.30% on average, and the unbound aggregates with a mean value of 28.17%.
Materials 2014, 7
However, as it can be observed in Table 1 and Figure 2, there is a wide variation in the composition between the different samples. The percentage of concrete content (natural aggregate and attached mortar) ranged between 12.76% and 56.41%, the natural aggregates without cement attached ranged between 9.33% and 45.44%, and ceramic particles content ranged between 16.51% and 64.75%. Glass content was lower than 1% for all the recycled aggregates. Asphalt content was lower than 4.50% for all samples, thus, no significant problems should be expected, since some studies [23,24] indicate that decrease of the compressive strength is due to a higher content of asphalt. In terms of gypsum content, the values ranged between 0.09% and 4.12%, which could generate some problems, specifically in Samples CDW2, CDW10, and CDW12, since, in a study conducted by Agrela et al. , it was found that recycled aggregates with a gypsum content, higher than 1.67%, should be rejected due to the lack of compliance with the 0.8% content limit for soluble sulphates in acid established in the Spanish and European specifications. Figure 2. Boxplots showing the different components of the recycled aggregates.
Lastly, some of the recycled aggregates (CDW2, CDW6, CDW7, CDW8, CDW10, CDW12, and CDW13) contained more than 1% of impurities (X1 + X2), thus, a pretreatment to remove the mentioned contaminations is necessary in order to comply with the EHE-08 requirements. This determination of the component proportions in the recycled coarse aggregates allowed a classification based on its ceramic content. Two groups of CDW treatment plants were established according to the following limits of ceramic particles contents in weight: • •
MixRA: samples with ceramic content inferior to 30%. Six facilities produce this type of recycled aggregate (CDW1, CDW3, CDW5, CDW8, CDW12, and CDW13). CerRA: samples with ceramic content superior to 30%. The rest of the CDW treatment plants produce this type of recycled aggregate (CDW2, CDW4, CDW6, CDW7, CDW10, and CDW11).
Materials 2014, 7
4.2. Physical-Mechanical Properties However, the previous study of composition and classification of the recycled aggregates did not determine the suitability of the material for its use in the manufacturing of concrete, being that the technical quality of the material is what determines its suitability. Therefore, Table 2 shows the results obtained for the tests conducted, and Figures 3 and 4 illustrate the margin in which the results fluctuate. Figure 3. Boxplots showing the fine content (F.C), sand equivalent (S.E), water absorption (W.A), flakiness index (F.I), and Los Angeles test value (L.A) of the recycled aggregates.
Figure 4. Boxplots showing the apparent density (ρa), after oven-drying density (ρrd), and saturated surface density (ρssd) of the recycled aggregates.
Materials 2014, 7
Table 2. Results of the physical-mechanical test conducted according to the EHE-08 . D: maximum particle size; d: minimum particle size; D/d: particle size ratio; F.C: fine content; S.E: sand equivalent; ρa: apparent density; ρrd: after oven-drying density; ρssd: saturated surface density; W.A: water absorption; F.I: flakiness index; and L.A: Los Angeles test value. Sample CDW1 CDW2 CDW3 CDW4 CDW5 CDW6 CDW7 CDW8 CDW9 CDW10 CDW11 CDW12 CDW13 Mean Standard deviation Maximum Minimum
D (mm) 31.50 31.50 31.50 31.50 31.50 12.50 20.00 31.50 31.50 31.50 31.50 12.50 12.50 26.23 8.44 31.5 12.5
d (mm) 10.00 0.40 0.40 0.32 1.25 0.06 4.00 2.00 2.00 16.00 10.00 4.00 4.00 4.19 4.88 16 0.06
D/d 3.15 78.75 78.75 100.00 25.20 198.40 5.00 15.80 15.80 1.97 3.20 3.10 3.10 40.94 58.58 198.4 1.97
F.C (%) 1.82 2.84 4.08 1.28 0.60 7.09 0.04 0.78 0.44 0.28 0.80 1.42 1.54 1.77 1.95 7.09 0.04
S.E (%) 35.40 20.80 65.90 48.30 49.00 38.80 38.10 45.30 26.70 43.27 11.5 38.10 34.50 38.13 13.64 65.9 11.5
ρa (Mg/m3) 2.57 2.60 2.65 2.56 2.58 2.58 2.59 2.64 2.56 2.58 2.62 2.66 2.68 2.61 0.04 2.68 2.56
ρrd (Mg/m3) 2.14 2.28 2.29 2.07 2.13 1.91 2.00 2.32 2.16 1.97 2.07 2.16 2.09 2.12 0.12 2.32 1.91
ρssd (Mg/m3) 2.31 2.28 2.43 2.26 2.30 2.17 2.23 2.44 2.32 2.21 2.28 2.35 2.31 2.30 0.08 2.44 2.17
W.A (%) 7.84 9.40 5.96 9.11 8.14 13.46 11.31 5.21 7.27 12.09 10.27 8.65 10.42 9.16 2.36 13.46 5.21
F.I (%) 14.94 29.57 24.67 12.25 9.61 4.64 14.75 11.98 11.85 16.67 42.13 7.07 7.36 15.96 10.48 42.13 4.64
L.A (%) 49.64 46.61 33.23 31.27 37.85 38.47 40.99 35.54 35.96 50.20 33.14 33.21 36.76 38.68 6.38 50.2 31.27
Materials 2014, 7
4.2.1. Particle Size Curves Particle size distributions of the MixRA and CerRA are shown in Figures 5 and 6, respectively. Figure 5. Particle size distribution curves of mixed recycled aggregates (MixRA).
Figure 6. Particle size distribution curves of ceramic recycled aggregates (CerRA).
Materials 2014, 7
The size distribution curves of all materials are continuous and non-uniform, indicating that the granulometry of the aggregate is correct in all sizes, which allows a greater margin for interaction between the particles and produces a greater degree of compactness and mechanical strength in the concrete . As indicated in the general requirements of the EHE-08 , Table 2 shows the maximum (D) and minimum (d) size of aggregates, and also depicts the relationship between both sizes. The D/d ratio is greater than 1.4, the limit stipulated in the EHE-08, for all the samples. However, since the EHE-08  defines coarse aggregate as particles with a minimum size of 4 mm, pretreatment of those samples, which do not meet this requirement, will be necessary (sieving to separate fines) before they can be employed as aggregate in concrete mixes. 4.2.2. Fine Content The EHE-08  establishes the need to study the quantity of fines (F.C), placing an upper limit of 1.5% for coarse aggregates. This is an extremely important test, since a high amount of fines would prevent good paste adhesion and encourage concrete failure . The results obtained, shown in Table 2, indicated that five of the samples (CDW1, CDW2, CDW3, CDW6, and CDW13) did not meet requirements. Nevertheless, the EHE-08  allows their use under the restrictions imposed in Article 31.1 Furthermore, Etxeberria et al.  recommended that a maximum limit for recycled aggregate fines of between 2% and 5% should not be exceeded, and all the samples tested fell below this limit, with the exception of CDW6, which would need to be pre-treated through sieving to reduce the fine fraction in the sample. 4.2.3. Sand Equivalent In the assessment of the fines, it is also necessary to test its quality, understood as the presence of fine clays, which is measured with the sand equivalent test (S.E). According to the class of exposure to which the concrete will be subjected, the values should exceed 70% or 75%. None of the samples complied with the limits established in the standard due to the presence of mortars and ceramic elements, which behave as clays, as indicated in Appendix 15 of the EHE-08 . Nevertheless, if the particle size of samples is adjusted for strict consideration as coarse aggregate (>4 mm), this restriction could be avoided. 4.2.4. Density Although the EHE-08 does not establish limits for any type of density—apparent (ρa), after oven-drying (ρrd) and saturated surface (ρssd), these are essential physical properties in the concrete mix design. The International Union of Laboratories and Experts in Construction Materials, Systems and Structures (RILEM)  recommends that if dry particles come from building rubble, they should have a minimum density of 1.5 Mg/m3. As can be seen in Table 2, all the samples presented densities which varied within the same ranges as those obtained for other ceramic materials from 1.6 Mg/m3 to 2.65 Mg/m3 in a study carried out by Sánchez de Juan and Alaejos , and exceeded the value recommended.
Materials 2014, 7
Interestingly, the density of recycled aggregates was significantly lower than that of the natural aggregates, which ranged between 2.4 Mg/m3 and 3 Mg/m3; this difference is explained by the greater porosity of recycled aggregate, due both to its ceramic nature and the presence of adhered mortar . This will imply an increased need for water and cement, rendering it more difficult to achieve the required levels of strength and durability in concrete [4,7,29]. 4.2.5. Water Absorption In contrast, water absorption is limited in the EHE-08  is up to 7% for recycled coarse aggregate. The determination of water absorption is a good indicator of the quality of the recycled aggregates, since these kinds of aggregates have a high absorption capacity that can be detrimental to the workability of the concrete mix [6,9]. In view of the results obtained (Table 4), which are similar to those reported by Agrela et al. , Mas et al.  and Barbudo et al. , only two of the aggregates studied would be suitable as partial replacement of the natural coarse aggregate (CDW3 and CDW8) since the rest do not comply with standard specifications. A higher absorption coefficient was observed with the increase in the percentage of masonry, which agreed with the findings of Gomes and de Brito . However, there is the possibility of using them if pre-treated by saturation with water before incorporating them into concrete mixes , which would involve using 5% more water according to Etxeberria et al. . Moreover, if the recycled aggregates were judged according to the RILEM  recommendations of a 20% limit all the samples would comply. 4.2.6. Shape In terms of shape, recycle aggregates from the CDW possess a different external morphology to that of natural aggregates, presenting sharp edges, angular outlines, variable shapes and a more or less flat surface, which can be seen with the naked eye. This external appearance is due both to the initial form of the waste (i.e., bricks, tiles…) and the process of obtaining the aggregate through use of a jaw crusher. Consequently, this type of secondary aggregate exhibits higher flakiness index than natural aggregates , which could lead to a reduction in the quality of the concrete in terms of lower strength and durability, since the need for a large quantity of water, cement, and sand, worsens workability . The shape of the coarse aggregates was determined by calculating the flakiness index as the percentage by weight of flaky and needle-like aggregates is obtained, which should be less than 35% since higher values would make it difficult to achieve high strength concretes. Table 4 shows the results obtained. The values obtained were in agreement with those reported by Mas et al. , except for one case, CDW11, the flakiness index values comply with the specifications given in the EHE-08 . Given that there is a narrow margin for non-compliance, and that the non-compliance was due to the large quantity of ceramic waste in the form of bricks contained in the sample and to the plant treatment method, one possible solution may lie in employing a different crushing procedure, as it was observed that other samples with the next higher percentages of ceramic waste (CDW6 and CDW10) did not present this problem.
Materials 2014, 7
4.2.7. Resistance to Fragmentation The EHE-08  recommends the use of the Los Angeles test to assess resistance to erosion of coarse aggregates through abrasion, wear, and impact, setting a value of 40% as the limit. Although the Los Angeles test has been identified by several authors [34,35] as a constraint property in the use of CDW, since the presence of ceramic and mortar implies less resistance to fragmentation , the results obtained (Table 4), which are similar to those reported by Mas et al.  and Vegas et al. , show that only CDW1, CDW2, CDW7, and CDW10 exceeded the limit of 40%. However, since only CDW10 exceed the 50% limit, the EHE-08 permits the use of the rest of them in concrete with a resistance lower than 30 N/mm2 if there are experimental studies to support such use. 4.2.8. Overall Performance Although recycled concrete aggregates are commonly considered the best option for a partial replacement of the natural coarse aggregate in the concrete manufacture, a recent study by Silva et al.  revealed that MixRA may have similar or even better physical properties for use in concrete and proposed a classification system, based on the recycled aggregates composition, but mostly on their physical properties. Following the aforementioned the performance-based aggregate classification system, the overall performance of the recycled aggregates was assessed (Table 3). Table 3. Performance-based classification of the recycled aggregates . Sample CDW1 CDW2 CDW3 CDW4 CDW5 CDW6 CDW7 CDW8 CDW10 CDW11 CDW12 CDW13
Class C C B C B C C B D C C C
Type I I II I III III II II I I I
As expected, the majority of recycled aggregates characterized belong to Class C and only one sample was included in Class D. Therefore, according to Silva et al.’s  recommendations, these aggregates should only be considered for use in low-grade applications (i.e., non-structural concrete). However, it is worth mentioning that as most of the aggregates failed the classification systems, hence, were included in a lower category, in terms of maximum water absorption (CDW2, CDW5, CDW6, CDW7, CDW12, and CDW13), an improvement could be achieved in their performance if some adjustments in the CDW treatment plant process were made. The results of a study  showed that, after the recycled aggregates were washed, the water absorption values fell by between 35% and 55% due to the removal of the finer particles. Consequently, the recycled aggregates obtained may be
Materials 2014, 7
susceptible to be used in higher-level applications with the addition of a relatively simple procedure in the treatment of the CDW. Additionally, three of the recycled aggregates studied (CDW3, CDW5 and CDW8), all of them previously classified as MixRA, belong to Class B, where most of the RCA could be placed, which indicate that some MixRA could present a high potential to be used in higher level applications, such as in partial replacement of the natural coarse aggregate in concrete manufacturing. 5. Conclusions The use of recycled aggregates from construction and demolition in the concrete manufacture requires that the secondary materials possess the sufficient technical requirements in order to qualify as a material for potential use in construction. Thus, a quality assessment was done by the comparison between the test results obtained and the limits established in the Spanish legislation to ensure the compliance. One of the problems with this approach is that recycled aggregates are characterized using traditional test methods, regardless of whether these are valid for the new materials. Consequently, establishing requirements for recycled aggregates on the basis of tests that may not be appropriate leaves these materials at a distinct disadvantage compared to conventional aggregates and creates a barrier to their use. Even so, and albeit the use of MixRA or CerRA has yet to be allowed by Spanish legislation, the results obtained for the characterization demonstrate that the untreated recycled aggregate samples with different ceramic contents (MixRA and CerRA) shows promising values for their use in concrete manufacturing if some simple pretreatments are carried out to fix some quality issues. Nonetheless, it is necessary to emphasize that the results obtained are the product of an analysis of the recycled aggregates from CDW, collected at a specific day of sampling, in each of the CDW treatment facilities, thus, the reproducibility over time within the same management plant is not ensured; although similar results should be expected if recycled aggregates with a similar composition are tested. In terms of composition, some of samples present a problem with the content of impurities, as the gypsum content reported could cause a non-compliance drawback with the requirements of soluble sulphates in acid that could be solved by carrying out a pretreatment of manual elimination of gypsum, which, as well, will remedy the problem of samples with a presence of impurities content over 1%. The physical-mechanical characterization shows that the untreated recycled aggregates complied in terms of particle size distribution, particle size, density, shape, and resistance to fragmentation with the requirements stipulated in the EHE-08 for use as a coarse aggregate in the manufacture of concrete. For the rest of parameters which the recycled aggregates presented a deviation with regard to the regulatory limits, as it is the case for fines and water absorption, a solution could be found by carrying out a pre-treatment to adjust particle size and water saturation of the recycled aggregate. Finally, some non-fulfillments, i.e., flakiness index and resistance to fragmentation, are impossible to alleviate by means of a pre-treatment and the recycled aggregate should be rejected for its use in concrete mixes but could be used in low level applications. In conclusion, although the absence of specific legislation permitting its use, if controlled the production process in the CDW treatment plant and pretreated previous to its use in the concrete mix
Materials 2014, 7
this type of recycled aggregate of ceramic origin has enough quality to become an input in the production of structural concrete. Acknowledgments This article was made possible by the University Teacher Training Grant (FPU AP2010-0613) and the Research Staff Training Grant (FPI BES-2011-047159) associated with Project BIA2010-21194-C03-02. Author Contributions Desirée Rodríguez-Robles and Julia García-González carried out the laboratory tests, and Andrés Juan-Valdés, Julia Mª Morán-del Pozo and M. Ignacio Guerra-Romero have controlled the whole project. Conflicts of Interest The authors declare no conflict of interest. References 1.
2. 3. 4.
5. 6. 7.
Schultmann, F.; Hiete, M.; Kuehlen, A.; Ludwig, J.; Schulte Beerbuehl, S.; Stengel, J.; Vannieuwenhuyse, M. Collection of Background Information for the Development of EMAS Pilot Reference Sectoral Documents: The Construction Sector; French-German Institute for Environmental Research (DFIU), Karlsruhe Institute of Technology (KIT): Karlsruhe, Germany, 2010. The European Environment State and Outlook 2010. Material Resources and Waste; European Environment Agency (EEA): Copenhagen, Denmark, 2010. Spanish Guide of Recycled Aggregates from CDW; Spanish DCW Management Association (GERD): Madrid, Spain, 2012. Etxeberria, M.; Barra, M.; Vazquez, E. Utilización de árido Reciclado para la Fabricación de Hormigón Estructural; Universitat Politècnica de Catalunya, Asociación Científico-Técnica del Hormigón Estructural: Barcelona, Spain, 2003. (In Spanish) Sánchez de Juan, M.; Alaejos, P. Influencia del árido reciclado en las propiedades del hormigón estructural (in Spanish). Cem. Hormig. 2006, 889, 54–61. Rao, A.; Jha, K.N.; Misra, S. Use of aggregates from recycled construction and demolition waste in concrete. Resour. Conserv. Recycl. 2007, 50, 71–81. Tam, V.W.Y.; Wang, K.; Tam, C.M. Assessing relationship among properties of demolished concrete, recycled aggregate and recycled aggregate concrete using regression analysis. J. Hazard. Mater. 2008, 152, 703–714. Martin-Morales, M.; Zamorano, M.; Ruiz-Moyano, A.; Valverde-Espinosa, I. Characterization of recycled aggregates construction and demolition waste for concrete production following the Spanish Structural Concrete Code EHE-08. Constr. Build. Mater. 2011, 25, 742–748. Agrela, F.; Sánchez de Juan, M.; Ayuso, J.; Geraldes, V.L.; Jiménez, J.R. Limiting properties in the characterisation of mixed recycled aggregates for use in the manufacture of concrete. Constr. Build. Mater. 2011, 25, 3950–3955.
Materials 2014, 7
10. Mas, B.; Cladera, A.; del Olmo, T.; Pitarch, F. Influence of the amount of mixed recycled aggregates on the properties of concrete for non-structural use. Constr. Build. Mater. 2012, 27, 612–622. 11. Code on Structural Concrete, EHE-08, Permanent Commission of the Concrete; Spanish Ministry of Public Works: Madrid, Spain, 2008. 12. De Brito, J.; Pereira, A.S.; Correia, J.R. Mechanical behaviour of non-structural concrete made with recycled ceramic aggregates. Cem. Concr. Compos. 2005, 27, 429–433. 13. National Plan of Construction and Demolition Waste 2001–2006, Resolution of 14 June, Boletín Oficial del Estado (BOE) N° 166; BOE: Madrid, Spain, 2001. 14. Google. Google Maps. Available online: https://www.google.com/maps/place/Spain (accessed on 15 July 2014). 15. Aggregates for Concrete; UNE-EN 12620:2003 + A1:2009; Spanish Association for Standardisation and Certification (AENOR): Madrid, Spain, 2009. 16. Test for General Properties of Aggregates. Part 1: Methods for Sampling; UNE-EN 932-1:1997; Spanish Association for Standardisation and Certification (AENOR): Madrid, Spain, 1997. 17. Tests for Geometrical Properties of Aggregates—Part 11: Classification Test for the Constituents of Coarse Recycled Aggregate; UNE-EN 933-11:2009/AC:2010; Spanish Association for Standardisation and Certification (AENOR): Madrid, Spain, 2010. 18. Tests for Geometrical Properties of Aggregates—Part 1: Determination of Particle Size Distribution—Sieving Method; UNE-EN 933-1:2012; Spanish Association for Standardisation and Certification (AENOR): Madrid, Spain, 2012. 19. Tests for Geometrical Properties of Aggregates—Part 8: Assessment of Fines—Sand Equivalent Test; UNE-EN 933-8:2012; Spanish Association for Standardisation and Certification (AENOR): Madrid, Spain, 2012. 20. Tests for Geometrical Properties of Aggregates—Part 3: Determination of Particle Shape—Flakiness Index; UNE-EN 933-3:2012; Spanish Association for Standardisation and Certification (AENOR): Madrid, Spain, 2012. 21. Tests for Mechanical and Physical Properties of Aggregates—Part 6: Determination of Particle Density and Water Absorption; UNE-EN 1097-6:2001/A1:2006; Spanish Association for Standardisation and Certification (AENOR): Madrid, Spain, 2006. 22. Tests for Mechanical and Physical Properties of Aggregates—Part 2: Methods for the Determination of Resistance to Fragmentation; UNE-EN 1097-2:2010; Spanish Association for Standardisation and Certification (AENOR): Madrid, Spain, 2010. 23. Guerra, I.; Vivar, I.; Llamas, B.; Juan, A.; Moran, J. Eco-efficient concretes: the effects of using recycled ceramic material from sanitary installations on the mechanical properties of concrete. Waste Manag. 2009, 29, 643–646. 24. Binici, H. Effect of crushed ceramic and basaltic pumice as fine aggregates on concrete mortars properties. Constr. Build. Mater. 2007, 21, 1191–1197. 25. Kraemer, C.; Pardillo, J.M.; Rocci, S.; Romana, M.G.; Sánchez Blanco, V.; del Val, M.A. Ingeniería de carreteras; McGraw Hill: Madrid, Spain, 2004; Volume 2. (In Spanish) 26. Fueyo, L. Equipos de Trituración, Molienda y Clasificación: Tecnología, Diseño y Aplicación; Rocas y Minerales: Madrid, Spain, 2002. (In Spanish)
Materials 2014, 7
27. The International Union of Laboratories and Experts in Construction Materials, Systems and Structures (RILEM) Recommendation. Specifications for concrete with recycled aggregates. Mater. Struct. 1994, 27, 557–559. 28. Poon, C.S.; Chan, D. Feasible use of recycled concrete aggregates and crushed clay brick as unbound road sub-base. Constr. Build. Mater. 2006, 20, 578–585. 29. Padmini, A.K.; Ramamurthy, K.; Mathews, M.S. Influence of parent concrete on the properties of recycled aggregate concrete. Constr. Build. Mater. 2009, 23, 829–836. 30. Barbudo, A.; Agrela, F.; Ayuso, J.; Jiménez, J.R.; Poon, C.S. Statistical analysis of recycled aggregates derived from different sources for sub-base applications. Constr. Build. Mater. 2012, 28, 129–138. 31. Gomes, M.; de Brito, J. Structural concrete with incorporation of coarse recycled concrete and ceramic aggregates: Durability performance. Mater. Struct. 2009, 42, 663–675. 32. Etxeberria, M.; Vázquez, E.; Marí, A.; Barra, M. Influence of amount of recycled coarse aggregates and production process on properties of recycled aggregate concrete. Cem. Concr. Res. 2007, 37, 735–742. 33. Zega, C.J.; Villagrán-Zaccardi, Y.A.; di Maio, A.A. Effect of natural coarse aggregate type on the physical and mechanical properties of recycled coarse aggregates. Mater. Struct. 2010, 43, 195–202. 34. Vegas, I.; Ibañez, J.A.; San Jose, J.T.; Urzelai, A. Construction demolition wastes, Waelz slag and MSWI bottom ash: A comparative technical analysis as material for road construction. Waste Manag. 2008, 28, 565–574. 35. Jiménez, J.R.; Agrela, F.; Ayuso, J.; López, M. A comparative study of recycled aggregates from concrete and mixed debris as material for unbound road sub-base. Mater. Constr. 2011, 61, 289–302. 36. Vegas, I.; Ibañez, J.A.; Lisbona, A.; Sáez de Cortazar, A.; Frías, M. Pre-normative research on the use of mixed recycled aggregates in unbound road sections. Constr. Build. Mater. 2011, 25, 2674–2682. 37. Silva, R.V.; de Brito, J.; Dhir, R.K. Properties and composition of recycled aggregates from construction and demolition waste suitable for concrete production. Constr. Build. Mater. 2014, 65, 201–217. 38. Van Der Wegen, G.; Haverkort, R. Recycled construction and demolition waste as a fine aggregate for concrete. In Proceedings of the International Symposium on Sustainable Construction: Use of Recycled Concrete Aggregate, London, UK, 11–12 November 1998; pp. 333–345. © 2014 by the authors; licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution license (http://creativecommons.org/licenses/by/3.0/).